Valence band offset of InN/BaTiO3 heterojunction measured by X-ray photoelectron spectroscopy
© Jia et al; licensee Springer. 2011
Received: 10 January 2011
Accepted: 8 April 2011
Published: 8 April 2011
X-ray photoelectron spectroscopy has been used to measure the valence band offset of the InN/BaTiO3 heterojunction. It is found that a type-I band alignment forms at the interface. The valence band offset (VBO) and conduction band offset (CBO) are determined to be 2.25 ± 0.09 and 0.15 ± 0.09 eV, respectively. The experimental VBO data is well consistent with the value that comes from transitivity rule. The accurate determination of VBO and CBO is important for use of semiconductor/ferrroelectric heterojunction multifunctional devices.
The semiconductor-ferroelectric heterostructures have attracted much attention due to their large potential for new multifunctional electronic and optoelectronic device applications [1–5]. Hysteresis properties of the ferroelectric polarization allow for bistable interface polarization configuration The polarization coupling between the fixed permanent semiconductor dipole and the switchable ferroelectric dipole can be exploited to modify the electronic and the optical properties of a semiconductor heterostructure. Recently, GaN-based high electron mobility transistor devices have been integrated on ferroelectric LiNbO3, providing the compact optoelectronic/electronic chips with increased cost savings and added functionality . The semiconductor-ZnO/ferroelectric-BaTiO3 (BTO) heterostructure metal-insulator-semiconductor field-effect transistors have been demonstrated, in which the polarization of the BTO can be used to control the free carrier concentration in the ZnO channel . In order to fully exploit the advantages of semiconductor-ferroelectric heterostructures, other combinations such as InN/BTO should be explored. As a remarkable ferroelectric material with a high relative permittivity, BTO can be used as a gate dielectric for InN-based field-effect transistor. More importantly, InN/BTO heterojunction is promising for fabricating optical and electrical devices since oxidation treatment is found to reduce the surface electron accumulation of InN films .
For heterostructure devices, it is important to accurately determine the valence and the conduction band offsets, which dictate the degree of charge carrier separation and localization. However, up to date, there is lack of experiment data available on the interface band alignment parameters for InN/BTO heterojunction. In this letter, we determine the VBO as well as conduction band offset (CBO) values of the InN/BTO heterojunction using X-ray photoelectron spectroscopy (XPS).
Three samples (bulk BTO, thick InN/BTO, and thin InN/BTO) were studied in this work, namely, a bulk commercial (001) BTO substrate, a thick 200-nm InN layer and a thin 5-nm InN layer grown on the commercial (001) BTO substrates, respectively. To get a clean interface, the BTO substrate was cleaned with organic solvents and rinsed with de-ionized water sequentially before loading into the reactor. The thick and thin heterostructures of InN/BTO were deposited by metal-organic chemical vapor deposition (MOCVD) at 520°C. More growth condition details of the InN layer can be found in our previous report . XPSs were performed on a PHI Quantera SXM instrument with Al Kα (hν = 1486.6 eV) as the X-ray radiation source, which had been carefully calibrated on work function and Fermi energy level (E F). Because a large amount of electrons are excited and emitted from the sample, the sample is always positively charged and the electric field caused by the charge can affect the measured kinetic energy of photoelectron. Charge neutralization was performed with an electron flood gun and all XPS spectra were calibrated by the C1s peak at 284.8 eV from contamination to compensate the charge effect. Since only the relative energy position in each sample is needed to determine the VBO, the absolute energy calibration for a sample has no effect on the ultimate result. The surfaces of samples were examined initially by low-resolution survey scans to determine which elements were present. Very high-resolution spectra were acquired to determine the binding energy of core level and the valence band maximum energy in the survey spectra.
Results and discussion
where is the energy difference between In3d and Ti2p core levels (CLs) measured in the thin heterojunction InN/BTO, while and are the valence band maximum (VBM) energies with reference to the CL positions of bulk BTO and thick InN film, respectively. Because all the samples were exposed to air, there must be some impurities (e.g., oxygen and carbon) existing in the sample surface, which may prevent the precise determination of the positions of the VBMs. To reduce the undesirable effects of surface contamination, all the samples were cleaned by Ar+ bombardment at a low sputtering rate to avoid damage to the samples. After the bombardment, peaks related to impurities were greatly reduced, and no new peaks appeared.
For the In3d spectra of both the InN and the thin InN/BTO samples, additional low intensity higher-binding-energy components were required. These extra components are attributed to In-O bonding due to oxide contamination when InN is present at the surface , as shown in Figure 2a. In the thin InN/BTO sample shown in Figure 2c, they are attributed to In-O bonding at the InN/BTO interfaces, and/or inelastic losses to free carriers in the InN layer . The CL peak attributed to In-N bonding locates at 443.67 ± 0.03 and 443.98 ± 0.03 eV for thick InN and thin InN/BTO, respectively, as shown in Figure 2a, c. From Figure 2b, it can be clearly seen that the Ti2p peak in the bulk BTO is not symmetric and consists of two components by careful Voigt fitting. The prominent one located at 457.12 ± 0.03 eV is attributed to the Ti emitters within the BTO substrate, which have six bonds to oxygen atoms. The other one shifting by ~2 eV to a lower binding energy is attributed to TiOx suboxides on account of the TiO-terminated BTO initial surface . However, the Ti2p spectrum in the thin InN/BTO heterojunction is quite symmetric, indicating a uniform bonding state and the only peaks correspond to Ti-O bonds. It is interesting that the Ti2p peaks transform from asymmetry in bulk BTO to symmetry in the thin InN/BTO sample, as recently observed in the thin ZnO/BTO heterostructure . The VBM value of bulk BTO is determined to be 1.49 ± 0.06 eV using the linear method. The Fermi energy level of an insulator is expected to be located in the middle of the forbidden energy gap, so the VBM will be one-half of the band gap of insulators . For BTO, the VBM should be 1.55 eV calculated from the band gap of 3.1 eV , which is in good agreement with the measured value (1.49 ± 0.06 eV) in the present work. Using the same fitting methods mentioned above, the VBM value for the thick InN lms can be determined to be 0.24 eV, as shown in Figure 1e. Substituting the above values in Equation 1, the resulting VBO value is calculated to be 2.25 ± 0.09 eV.
The reliability of the measured result is analyzed by considering several possible factors that could impact the experiment results. The energy band bends downward at the surface of InN film and there is an electron accumulation layer , so the energy separation between VBM and Fermi level can be changed at the InN surface, which could impact the measured VBO values of the heterojunctions. However, both the CL emissions of In3d and Ti2p at the InN/BTO heterojunction are collected from the same surface (InN surface), thus, the surface band bending effects can be canceled out for the measurement of ΔE CL, as was the measurement of the band offset of the InN/AlN heterojunction by others [19, 20].
Another factor which may affect the precision of the VBO value is the strain-induced piezoelectric field in the overlayer of the heterojunction . There is a large lattice mismatch of about 7.1% between the hexagonal apothem of InN and the direction. It is comparable with that of the InN/ZnO heterojunction (7.7%), and the InN thin film of 5 nm is approximately treated as completely relaxed . So the strain-induced piezoelectric field effect can be neglected in our experiment. Since the factors that can affect the ultimate result can be excluded from the measured result, the experimental obtained VBO value is somewhat reliable.
To further confirm the reliability of the experimental values, it would be useful to compare our VBO value with other results deduced by transitive property. For heterojunctions formed between all pairs of three materials (A, B, and C), ΔE V(A-C) can be deduced from the difference between ΔE V(A-B) and ΔE V(C-B) neglecting the interface effects . The reported VBO values for ZnO/BTO and InN/ZnO heterojunctions are ΔE V(ZnO-BTO) = 0.48 eV , and ΔE V(InN-ZnO) = 1.76 eV , respectively. Then the ΔE V(InN-BTO) is deduced to be 2.24 eV, which is well consistent with our measured value 2.25 ± 0.09 eV. In addition, the resulting ΔE V is a large value for device applications which require strong carrier con nement, such as light emitters or heterostructure field effect transistors.
In summary, XPS was used to measure the VBO of the InN/BTO heterojunction. A type-I band alignment with the VBO of 2.25 ± 0.09 eV and CBO of 0.15 ± 0.09 eV is obtained. The accurately determined result is important for the design and application of InN/BTO heterostructure-based devices.
conduction band offset
metal-organic chemical vapor deposition
valence band maximum
valence band offset
X-ray photoelectron spectroscopy.
This work was supported by the 973 program (2006CB604908, 2006CB921607), and the National Natural Science Foundation of China (60625402, 60990313).
- Voora VM, Hofmann T, Schubert M, Brandt M, Lorenz M, Grundmann M, Ashkenov N, Schubert M: Resistive hysteresis and interface charge coupling in BaTiO 3 -ZnO heterostructures. Appl Phys Lett 2009, 94: 142904. 10.1063/1.3116122View ArticleGoogle Scholar
- Voora VM, Hofmann T, Brandt M, Lorenz M, Grundmann M, Ashkenov N, Schmidt H, Ianno N, Schbert M: Interface polarization coupling in piezoelectric-semiconductor ferroelectric heterostructures. Phys Rev B 2010, 81: 195307. 10.1103/PhysRevB.81.195307View ArticleGoogle Scholar
- Mbenkum BN, Ashkenov N, Schubert M, Lorentz M, Hochmuth H, Michel D, Grundmann M, Wagner G: Temperature-dependent dielectric and electro-optic properties of a ZnO-BaTiO 3 -ZnO heterostructure grown by pulsed-laser deposition. Appl Phys Lett 2005, 86: 091904. 10.1063/1.1862778View ArticleGoogle Scholar
- Losego MD, Kourkoutis LF, Mita S, Craft HS, Muller DA, Collazo R, Sitar Z, Maria JP: Epitaxial Ba 0.5 Sr 0.5 TiO 3 -GaN heterostructures with abrupt interfaces. J Cryst Growth 2009, 311: 1106. 10.1016/j.jcrysgro.2008.11.085View ArticleGoogle Scholar
- Lorentz M, Brandi M, Schubert J, Hochmuth H, v Wenckstern H, Schubert M, Grundmann M: Polarization coupling in epitaxial ZnO/BaTiO 3 thin film heterostructures on SrTiO 3 (100) substrates. Proc SPIE 2007, 6474: 64741S.View ArticleGoogle Scholar
- Namkoong G, Lee KK, Madison SM, Henderson W, Doolittle WA, Ralph SE: III-nitride integration on ferroelectric materials of lithium niobate by molecular beam epitaxy. Appl Phys Lett 2005, 87: 171107. 10.1063/1.2084340View ArticleGoogle Scholar
- Brandt M, Frenzel H, Hochmuth H, Lorentz M, Grundmann M, Schubert J: Ferroelectric thin film field-effect transistors based on ZnO/BaTiO 3 heterostructures. J Vac Sci Technol B 2009, 27: 1789. 10.1116/1.3086720View ArticleGoogle Scholar
- Cimalla V, Lebedev V, Wang CY, Ali M, Cke GE, Polyakov VM, Schwierz F, Ambacher O, Lu H, Scha WJ: Reduced surface electron accumulation at InN films by ozone induced oxidation. Appl Phys Lett 2007, 90: 152106. 10.1063/1.2721365View ArticleGoogle Scholar
- Jia CH, Chen YH, Zhou XL, Liu GH, Guo Y, Liu XL, Yang SY, Wang ZG: InN layers grown by MOCVD on SrTiO 3 substrates. J Cryst Growth 2010, 312: 373. 10.1016/j.jcrysgro.2009.10.066View ArticleGoogle Scholar
- Zhang RQ, Zhang PF, Kang TT, Fan HB, Liu XL, Yang SY, Wei HY, Zhu QS, Wang ZG: Determination of the valence band offset of wurtzite InN/ZnO heterojunction by x-ray photoelectron spectroscopy. Appl Phys Lett 2007, 91: 162104. 10.1063/1.2800311View ArticleGoogle Scholar
- Chambers SA, Droubay T, Kaspar TC, Gutowski M: Experimental determination of valence band maxima for SrTiO 3 , TiO 2 , and SrO and the associated valence band offsets with Si(001). J Vac Sci Technol B 2004, 22: 2205. 10.1116/1.1768525View ArticleGoogle Scholar
- Piper LFJ, Veal TD, Walker M, Mahboob I, Mcconville CF, Lu H, Scha WJ: Clean wurtzite InN surfaces prepared with atomic hydrogen. J Vac Sci Technol A 2005, 23: 617. 10.1116/1.1927108View ArticleGoogle Scholar
- King PDC, Veal TD, Lu H, Hatfield SA, Schaff WJ, Mcconville CF: The influence of conduction band plasmons on core-level photoemission spectra of InN. Surf Sci 2008, 602: 871. 10.1016/j.susc.2007.12.026View ArticleGoogle Scholar
- Kazzi ME, Merckling C, Delhaye G, Arzel L, Grenet G, Bergignat E, Hollinger G: Photoemission (XPS and XPD) study of epitaxial LaAlO 3 film grown on SrTiO 3 (0 0 1). Mater Sci Semicond Process 2006, 9: 954. 10.1016/j.mssp.2006.10.044View ArticleGoogle Scholar
- Jia CH, Chen YH, Zhou XL, Yang AL, Zheng GL, Liu XL, Yang SY, Wang ZG: Valence band offset of ZnO/BaTiO 3 heterojunction measured by X-ray photoelectron spectroscopy. Appl Phys A 2010, 99: 511. 10.1007/s00339-010-5599-yView ArticleGoogle Scholar
- You JB, Zhang XW, Song HP, Ying J, Guo Y, Yang AL, Yin ZG, Chen NF, Zhu QS: Energy band alignment of SiO 2 /ZnO interface determined by x-ray photoelectron spectroscopy. J Appl Phys 2009, 106: 043709. 10.1063/1.3204028View ArticleGoogle Scholar
- Boggess TF, White JO, Valley GC: Two-photon absorption and anisotropic transient energy transfer in BaTiO 3 with 1-psec excitation. J Opt Soc Am B 1990, 7: 2255. 10.1364/JOSAB.7.002255View ArticleGoogle Scholar
- Mahboob I, Veal TD, Mcconville CF, Lu H, Scha WJ: Intrinsic Electron Accumulation at Clean InN Surfaces. Phys Rev Lett 2004, 92: 036804. 10.1103/PhysRevLett.92.036804View ArticleGoogle Scholar
- Wu CL, Shen CH, Gwo S: Valence band offset of wurtzite InN/AlN heterojunction determined by photoelectron spectroscopy. Appl Phys Lett 2006, 88: 032105. 10.1063/1.2165195View ArticleGoogle Scholar
- King PDC, Veal TD, Jefferson PH, Mcconville CF, Wang T, Parbrook PJ, Lu H, Scha WJ: Valence band offset of InN/AlN heterojunctions measured by x-ray photoelectron spectroscopy. Appl Phys Lett 2007, 90: 132105. 10.1063/1.2716994View ArticleGoogle Scholar
- Martin G, Botchkarev A, Rockett A, Morkoc H: Valence-band discontinuities of wurtzite GaN, AlN, and InN heterojunctions measured by x-ray photoemission spectroscopy. Appl Phys Lett 1996, 68: 2541. 10.1063/1.116177View ArticleGoogle Scholar
- Foulon Y, Priester C: Band-offset transitivity in strained (001) heterointerfaces. Phys Rev B 1992, 45: 6259. 10.1103/PhysRevB.45.6259View ArticleGoogle Scholar
- Yang AL, Song HP, Wei HY, Liu XL, Wang J, Lv XQ, Jin P, Yang SY, Zhu QS, Wang ZG: Measurement of polar C-plane and nonpolar A-plane InN/ZnO heterojunctions band offsets by x-ray photoelectron spectroscopy. Appl Phys Lett 2009, 94: 163301. 10.1063/1.3123814View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.